Time-resolved photoluminescence studies of annealed 1.3-μm GaInNAsSb quantum wells
© Baranowski et al.; licensee Springer. 2014
Received: 14 November 2013
Accepted: 3 February 2014
Published: 17 February 2014
Time-resolved photoluminescence (PL) was applied to study the dynamics of carrier recombination in GaInNAsSb quantum wells (QWs) emitting near 1.3 μm and annealed at various temperatures. It was observed that the annealing temperature has a strong influence on the PL decay time, and hence, it influences the optical quality of GaInNAsSb QWs. At low temperatures, the PL decay time exhibits energy dependence (i.e., the decay times change for different energies of emitted photons), which can be explained by the presence of localized states. This energy dependence of PL decay times was fitted by a phenomenological formula, and the average value of E0, which describes the energy distribution of localized states, was extracted from this fit and found to be smallest (E0 = 6 meV) for the QW annealed at 700°C. In addition, the value of PL decay time at the peak energy was compared for all samples. The longest PL decay time (600 ps) was observed for the sample annealed at 700°C. It means that based on the PL dynamics, the optimal annealing temperature for this QW is approximately 700°C.
KeywordsGaInNAsSb Quantum wells Time-resolved spectroscopy
Incorporation of small amounts of nitrogen into a GaInAs host causes a strong reduction of the energy gap as well as a reduction of the lattice constant. A few percent of nitrogen is enough to tune the energy gap of GaInNAs to the 1.3- and 1.55-μm spectral regions. Because of that, GaInNAs alloys have attracted much attention for low-cost GaAs-based lasers operating at II and III telecommunication windows[2–4]. However, the optical quality of Ga(In)NAs alloys strongly deteriorates with increasing nitrogen concentration due to phase segregation and the incorporation of point defects such as gallium interstitials, nitrogen interstitials[6, 7], arsenic antisites, and gallium vacancies. Post-growth annealing is the standard procedure to remove defects in an as-grown material to improve its optical quality[8, 9]. The optical quality of strained GaInNAs alloys can also be improved by adding antimony to form GaInNAsSb alloys with 2% to 3% Sb concentration. This is due to the reactive surfactant properties of antimony, which reduce the group III surface diffusion length suppressing phase segregation and roughening and thereby improving alloy homogeneity[10, 11]. The incorporation of antimony reduces the energy gap of the alloy, and hence, it is possible to reach longer emission wavelengths with lower nitrogen concentrations. Using GaInNAsSb quantum wells (QWs), lasers and vertical-cavity surface-emitting lasers operating at 1.3 μm and 1.55 μm[13, 14] have been demonstrated. However, the quality of an as-grown GaInNAsSb material can still be improved by post-growth annealing[15, 16]. The effects of annealing on the optical properties of GaInNAsSb QWs have been studied in detail (see, for example, and references therein). The annealing conditions for dilute nitrides are optimized based on the peak or integrated photoluminescence (PL) intensity. Recently, we demonstrated that the peak PL intensity in 1.3-μm GaInNAsSb QWs depends not only on the optical quality of the QW but also on the efficiency of carrier collection of the QW. In this paper, we applied time-resolved photoluminescence (TRPL) to investigate the carrier dynamics in GaInNAsSb QWs at low temperature and identify the optimal annealing conditions based on the parameters that describe the carrier dynamics.
The QW structures used in this study were grown by molecular beam epitaxy on (001) n-type GaAs substrates and consist of a 300-nm GaAs buffer layer, a 7.5-nm Ga0.66In0.34 N0.008As0.97Sb0.022 QW surrounded by 20-nm strain-compensating GaN0.008As0.992 barriers, and a 50-nm GaAs cap layer. It is worth noting that GaN0.008As0.992 barriers do not compensate the strain in the QW region, but they help improve the structural quality of the Ga0.66In0.34 N0.008As0.97Sb0.022 layer. After the growth, the samples were annealed for 60 s at different temperatures from 680°C to 800°C in 20°C steps. The growth conditions are similar to those used for a 1.55-μm GaInNAsSb QW and can be found elsewhere. For the TRPL experiment, the samples were held in a vapor helium cryostat allowing measurements at variable temperatures. They were excited by a mode-locked Ti:sapphire laser with a 76-MHz repetition rate and a pulse duration of 150 fs. The laser wavelength was set to 800 nm and its average excitation power density was approximately 3 W/cm2. The PL signal was dispersed by a 0.3-m-focal length monochromator, and the temporal evolution of the PL signal was detected by a streak camera with S1 photocathode while the time-integrated spectrum was recorded by an InGaAs CCD camera. The effective time resolution of the system is approximately 20 ps.
Results and discussion
Figure 1b shows τPL constants extracted by fitting the experimental data. It is clearly visible that the annealing temperature has a significant influence on the PL decay time. The τPL equals approximately 350 ps for the as-grown QW and increases after annealing to 600 ps for the QW annealed at 700°C. At higher annealing temperatures, τPL decreases with increasing annealing temperature reaching values comparable to the τPL of the as-grown QW for annealing temperatures in the 780°C to 800°C range.
The τPL constant is directly related to the optical quality of QW since τPL can be expressed in terms of the radiative (τr) and nonradiative (τnr) lifetimes according to the formula 1 / τPL = 1 / τr + 1 / τnr. The radiative lifetime is proportional to the wave function overlap which does not change significantly during annealing. Obviously, the annealing can cause some QW intermixing[19, 20], but this change in QW potential shape is too small to significantly reduce the wave function overlap. Therefore, any differences in τPL arise from differences in τnr. Stronger nonradiative recombination leads to shorter τnr and hence shorter τPL. From the TRPL studies (see Figure 1), we can conclude that the optimal annealing temperature (in the sense of the optical quality of the QW layer) is approximately 700°C as it yields the longest τPL. Annealing at higher temperatures creates defects that act as new centers of nonradiative recombination that degrade the optical quality of the QW. This conclusion is consistent with our room-temperature TRPL studies for this set of samples. It is worth noting that the low-temperature TRPL measurements presented in this work were performed at a relatively low excitation power density (3 W/cm2) to minimize the saturation of the localized states, which can obscure the differences between the samples annealed at different temperatures.
The values of E0 for the annealed 1.3-μm GaInNAsSb QWs are in the range of 6 to 7 meV. These values are comparable to the values of E0 for dilute nitrides reported in the literature: approximately 6 meV for a GaInNAs multiple QW structure with 1.5% of nitrogen and approximately 9 meV for a GaInNAs epilayer with 1% of nitrogen.
In conclusion, 1.3-μm GaInNAsSb QWs annealed at various temperatures (from 680°C to 800°C in 20°C steps) were studied by low-temperature TRPL. It has been shown that exciton dynamics in these QWs change significantly with annealing temperature. Due to carrier localization, strong energy dependence of the PL decay time is observed for all samples at low temperatures. This energy dependence was fitted by a phenomenological formula that assumes an exponential distribution of localized states. The average value of E0, which describes the energy distribution of localized states, has been extracted from this fit, and its dependence on annealing temperature was studied. The smallest value of E0 was observed for the GaInNAsSb QW annealed at 700°C. In addition, the PL decay time measured at the peak PL energy was compared for all samples. The longest PL decay time was also observed for the QW annealed at 700°C. Based on these parameters that describe the carrier dynamics at low temperature, it can be concluded that the optimal annealing temperature for this QW is approximately 700°C.
This work was performed within the grant of the National Science Centre (no. 2012/07/E/ST3/01742). MB acknowledges the support from the MNiSW within the Iuventus Plus program (IP2011 001471).
- Shan W, Walukiewicz W, Ager JW, Haller EE, Geisz JF, Friedman DJ, Olson JM, Kurtz SR: Band anticrossing in GaInNAs alloys. Phys Rev Lett 1999, 82: 1221–1224. 10.1103/PhysRevLett.82.1221View Article
- Choquette KD, Klem JF, Fischer AJ, Blum O, Allerman AA, Fritz IJ, Kurtz SR, Breiland WG, Sieg R, Geib KM, Scott JW, Naone RL: Room temperature continuous wave InGaAsN quantum well vertical-cavity lasers emitting at 1.3 μm. Electron Lett 2000, 36: 1388. 10.1049/el:20000928View Article
- Tansu N, Mawst LJ: Temperature sensitivity of 1300-nm InGaAsN quantum-well lasers. IEEE Photonics Technol Lett 2002, 14: 1052–1054.View Article
- Jaschke G, Averbeck R, Geelhaar L, Riechert H: Low threshold InGaAsN/GaAs lasers beyond 1500 nm. J Cryst Growth 2005, 278: 224–228. 10.1016/j.jcrysgro.2004.12.059View Article
- Wang XJ, Puttisong Y, Tu CW, Ptak AJ, Kalevich VK, Egorov AY, Geelhaar L, Riechert H, Chen WM, Buyanova IA: Dominant recombination centers in Ga(In)NAs alloys: Ga interstitials. Appl Phys Lett 2009, 95: 241904. 10.1063/1.3275703View Article
- Chen WM, Buyanova IA, Tu CW: Defects in dilute nitrides: significance and experimental signatures. Optoelectron IEE Proc 2004, 151: 379–384. 10.1049/ip-opt:20040939View Article
- Krispin P, Gambin V, Harris JS, Ploog KH: Nitrogen-related electron traps in Ga(As, N) layers (≤3% N). J Appl Phys 2003, 93: 6095–6099. 10.1063/1.1568523View Article
- Spruytte SG, Coldren CW, Harris JS, Wampler W, Krispin P, Ploog K, Larson MC: Incorporation of nitrogen in nitride-arsenides: origin of improved luminescence efficiency after anneal. J Appl Phys 2001, 89: 4401–4406. 10.1063/1.1352675View Article
- Pan Z, Li LH, Zhang W, Lin YW, Wu RH, Ge W: Effect of rapid thermal annealing on GaInNAs/GaAs quantum wells grown by plasma-assisted molecular-beam epitaxy. Appl Phys Lett 2000, 77: 1280–1282. 10.1063/1.1289916View Article
- Yang X, Jurkovic MJ, Heroux JB, Wang WI: Molecular beam epitaxial growth of InGaAsN:Sb/GaAs quantum wells for long-wavelength semiconductor lasers. Appl Phys Lett 1999, 75: 178–180. 10.1063/1.124311View Article
- Massies J, Grandjean N: Surfactant effect on the surface diffusion length in epitaxial growth. Phys Rev B 1993, 48: 8502–8505. 10.1103/PhysRevB.48.8502View Article
- Shimizu H, Setiagung C, Ariga M, Ikenaga Y, Kumada K, Hama T, Ueda N, Iwai N, Kasukawa A: 1.3-μm-range GaInNAsSb-GaAs VCSELs. IEEE J Sel Top Quantum Electron 2003, 9: 1214–1219. 10.1109/JSTQE.2003.819505View Article
- Bank SR, Bae H, Goddard LL, Yuen HB, Wistey MA, Kudrawiec R, Harris JS: Recent progress on 1.55-μm dilute-nitride lasers. IEEE J Quantum Electron 2007, 43: 773–785.View Article
- Sarmiento T, Bae HP, O'Sullivan TD, Harris JS: GaAs-based 1.53 μm GaInNAsSb vertical cavity surface emitting lasers. Electron Lett 2009, 45: 978. 10.1049/el.2009.1626View Article
- Kudrawiec R, Poloczek P, Misiewicz J, Bae HP, Sarmiento T, Bank SR, Yuen HB, Wistey MA, Harris JS Jr: Contactless electroreflectance of GaInNAsSb/GaNAs/GaAs quantum wells emitting at 1.5–1.65 μm: broadening of the fundamental transition. Appl Phys Lett 2009, 94: 031903. 10.1063/1.3073718View Article
- Bae HP, Bank SR, Yuen HB, Sarmiento T, Pickett ER, Wistey MA, Harris JS: Temperature dependencies of annealing behaviors of GaInNAsSb/GaNAs quantum wells for long wavelength dilute-nitride lasers. Appl Phys Lett 2007, 90: 231119. 10.1063/1.2746944View Article
- Baranowski M, Kudrawiec R, Latkowska M, Syperek M, Misiewicz J, Sarmiento T, Harris JS: Enhancement of photoluminescence from GaInNAsSb quantum wells upon annealing: improvement of material quality and carrier collection by the quantum well. J Phys Condens Matter 2013, 25: 065801. 10.1088/0953-8984/25/6/065801View Article
- Harris JS Jr, Kudrawiec R, Yuen HB, Bank SR, Bae HP, Wistey MA, Jackrel D, Pickett ER, Sarmiento T, Goddard LL, Lordi V, Gugov T: Development of GaInNAsSb alloys: growth, band structure, optical properties and applications. Phys Status Solidi B Basic Res 2007, 244: 2707–2729. 10.1002/pssb.200675620View Article
- Dixit V, Liu HF, Xiang N: Analysing the thermal-annealing-induced photoluminescence blueshifts for GaInNAs/GaAs quantum wells: a genetic algorithm based approach. J. Phys Appl Phys 2008, 41: 115103. 10.1088/0022-3727/41/11/115103View Article
- Liu HF, Dixit V, Xiang N: Anneal-induced interdiffusion in 1.3-μmGaInNAs/GaAs quantum well structures grown by molecular-beam epitaxy. J Appl Phys 2006, 99: 013503. 10.1063/1.2150259View Article
- Sun Z, Xu ZY, Yang XD, Sun BQ, Ji Y, Zhang SY, Ni HQ, Niu ZC: Nonradiative recombination effect on photoluminescence decay dynamics in GaInNAs/GaAs quantum wells. Appl Phys Lett 2006, 88: 011912. 10.1063/1.2161071View Article
- Kudrawiec R, Sęk G, Misiewicz J, Gollub D, Forchel A: Explanation of annealing-induced blueshift of the optical transitions in GaInAsN/GaAs quantum wells. Appl Phys Lett 2003, 83: 2772–2774. 10.1063/1.1615673View Article
- Lordi V, Yuen HB, Bank SR, Wistey MA, Harris JS, Friedrich S: Nearest-neighbor distributions in Ga1-xIn x N y As1-y and Ga1-xIn x N y As1-y-zSb z thin films upon annealing. Phys Rev B 2005, 71: 125309.View Article
- Buyanova IA, Chen WM, Pozina G, Bergman JP, Monemar B, Xin HP, Tu CW: Mechanism for low-temperature photoluminescence in GaNAs/GaAs structures grown by molecular-beam epitaxy. Appl Phys Lett 1999, 75: 501–503. 10.1063/1.124429View Article
- Kudrawiec R, Sek G, Misiewicz J, Li LH, Harmand JC: Investigation of recombination processes involving defect-related states in (Ga, In)(As, Sb, N) compounds. Eur Phys J Appl Phys 2004, 27: 313–316. 10.1051/epjap:2004056View Article
- Kaschner A, Lüttgert T, Born H, Hoffmann A, Egorov AY, Riechert H: Recombination mechanisms in GaInNAs/GaAs multiple quantum wells. Appl Phys Lett 2001, 78: 1391–1393. 10.1063/1.1355014View Article
- Baranovskii SD, Eichmann R, Thomas P: Temperature-dependent exciton luminescence in quantum wells by computer simulation. Phys Rev B 1998, 58: 13081–13087. 10.1103/PhysRevB.58.13081View Article
- Mair RA, Lin JY, Jiang HX, Jones ED, Allerman AA, Kurtz SR: Time-resolved photoluminescence studies of In x Ga1-xAs1-yN y . Appl Phys Lett 2000, 76: 188–190. 10.1063/1.125698View Article
- Zu LQ, Lin JY, Jiang HX: Dynamics of exciton localization in a CdSe0.5S0.5 mixed crystal. Phys Rev B 1990, 42: 7284–7287. 10.1103/PhysRevB.42.7284View Article
- Ouadjaout D, Marfaing Y: Thermal activation of localized excitons in Zn x Hg1-xTe semiconductor alloys: photoluminescence line-shape analysis. Phys Rev B 1992, 46: 7908–7910. 10.1103/PhysRevB.46.7908View Article
- Cho Y-H, Song JJ, Keller S, Minsky MS, Hu E, Mishra UK, DenBaars SP: Influence of Si doping on characteristics of InGaN/GaN multiple quantum wells. Appl Phys Lett 1998, 73: 1128–1130. 10.1063/1.122105View Article
- Cho Y-H, Gainer GH, Fischer AJ, Song JJ, Keller S, Mishra UK, DenBaars SP: "S-shaped" temperature-dependent emission shift and carrier dynamics in InGaN/GaN multiple quantum wells. Appl Phys Lett 1998, 73: 1370–1372. 10.1063/1.122164View Article
- Lin YC, Chung HL, Chou WC, Chen WK, Chang WH, Chen CY, Chyi JI: Carrier dynamics in isoelectronic ZnSe1-xO x semiconductors. Appl Phys Lett 2010, 97: 041909. 10.1063/1.3473776View Article
- Gourdon C, Lavallard P: Exciton transfer between localized states in CdS1–xSe x alloys. Phys Status Solidi B 1989, 153: 641–652. 10.1002/pssb.2221530222View Article
- Rubel O, Baranovskii SD, Hantke K, Kunert B, Rühle WW, Thomas P, Volz K, Stolz W: Model of temperature quenching of photoluminescence in disordered semiconductors and comparison to experiment. Phys Rev B 2006, 73: 233201.View Article
- Rubel O, Galluppi M, Baranovskii SD, Volz K, Geelhaar L, Riechert H, Thomas P, Stolz W: Quantitative description of disorder parameters in (GaIn)(NAs) quantum wells from the temperature-dependent photoluminescence spectroscopy. J Appl Phys 2005, 98: 063518–063518. –7 –7 10.1063/1.2058192View Article
- Grüning H, Kohary K, Baranovskii SD, Rubel O, Klar PJ, Ramakrishnan A, Ebbinghaus G, Thomas P, Heimbrodt W, Stolz W, Rühle WW: Hopping relaxation of excitons in GaInNAs/GaNAs quantum wells. Phys Status Solidi C 2004, 1: 109–112. 10.1002/pssc.200303604View Article
- Baranowski M, Latkowska M, Kudrawiec R, Misiewicz J: Model of hopping excitons in GaInNAs: simulations of sharp lines in micro-photoluminescence spectra and their dependence on the excitation power and temperature. J Phys Condens Matter 2011, 23: 205804. 10.1088/0953-8984/23/20/205804View Article
- Oueslati M, Benoit C, Zouaghi M: Resonant Raman scattering on localized states due to disorder in GaAs1-xP x alloys. Phys Rev B 1988, 37: 3037–3041. 10.1103/PhysRevB.37.3037View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.